| Sample no. | Composition (mol%) | Composition (mol%) | Composition (mol%) | T  g  (degC) | T  p  (degC) | T  p  (degC) | d (g/cm3) | n    |
| Sample no. | Gd2O3              | WO3                | B2O3               | T  g  (degC) | T  p  (degC) | T  p  (degC) | d (g/cm3) | n    |
| 1          | 25                 | 25                 | 50                 | 666          | 666          | 874          | 5.640     | 1.82 |
| 2          | 25                 | 30                 | 45                 | 654          | 654          | 888          | 5.662     | 1.83 |
| 3          | 25                 | 35                 | 40                 | 650          | 650          | 883          | 5.793     | 1.85 |
| 4          | 25                 | 40                 | 35                 | 640          | 640          | 850          | 5.929     | 1.86 |
| 5          | 25                 | 45                 | 30                 | 633          | 633          | 819          | 6.152     | 1.88 |
| 6          | 25                 | 50                 | 25                 | 631          | 631          | 783          | 6.326     | 1.90 |
| 7          | 25                 | 55                 | 20                 | 624          | 624          | 773          | 6.490     | 1.91 |
| 8          | 25                 | 60                 | 15                 | 614          | 614          | 752          | 6.617     | 1.93 |
| 9          | 25                 | 65                 | 10                 | 612          | 612          | 724          | 6.773     | 1.94 |

Caption: Chemical composition, the glass transition temperature (T g ), crystallization peak temperature (T p ), density (d), and refractive index (n) at 632.8nm for 25Gd2O3-(75-x)WO3-75B2O3 glasses with x=25-65. The experimental uncertainties of T g , T p , d, and n are +-2degC, +-2degC, +-0.003g/cm3, and +-0.01, respectively.

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "1", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "1"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "1"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "1"}
{"value": "666", "type": "Other"}
{"value": "666", "type": "Other"}
{"value": "874", "type": "Other"}
{"value": "5.640", "type": "Other"}
{"value": "1.82", "type": "Other"}
{"value": "2", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "2"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "2"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "2"}
{"value": "654", "type": "Other"}
{"value": "654", "type": "Other"}
{"value": "888", "type": "Other"}
{"value": "5.662", "type": "Other"}
{"value": "1.83", "type": "Other"}
{"value": "3", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "3"}
{"value": "35", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "3"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "3"}
{"value": "650", "type": "Other"}
{"value": "650", "type": "Other"}
{"value": "883", "type": "Other"}
{"value": "5.793", "type": "Other"}
{"value": "1.85", "type": "Other"}
{"value": "4", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "4"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "4"}
{"value": "35", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "4"}
{"value": "640", "type": "Other"}
{"value": "640", "type": "Other"}
{"value": "850", "type": "Other"}
{"value": "5.929", "type": "Other"}
{"value": "1.86", "type": "Other"}
{"value": "5", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "5"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "5"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "5"}
{"value": "633", "type": "Other"}
{"value": "633", "type": "Other"}
{"value": "819", "type": "Other"}
{"value": "6.152", "type": "Other"}
{"value": "1.88", "type": "Other"}
{"value": "6", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "6"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "6"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "6"}
{"value": "631", "type": "Other"}
{"value": "631", "type": "Other"}
{"value": "783", "type": "Other"}
{"value": "6.326", "type": "Other"}
{"value": "1.90", "type": "Other"}
{"value": "7", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "7"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "7"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "7"}
{"value": "624", "type": "Other"}
{"value": "624", "type": "Other"}
{"value": "773", "type": "Other"}
{"value": "6.490", "type": "Other"}
{"value": "1.91", "type": "Other"}
{"value": "8", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "8"}
{"value": "60", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "8"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "8"}
{"value": "614", "type": "Other"}
{"value": "614", "type": "Other"}
{"value": "752", "type": "Other"}
{"value": "6.617", "type": "Other"}
{"value": "1.93", "type": "Other"}
{"value": "9", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Gd2O3", "unit": "mol", "material": "9"}
{"value": "65", "type": "Glass_Compound_Amount", "constituent": "WO3", "unit": "mol", "material": "9"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "9"}
{"value": "612", "type": "Other"}
{"value": "612", "type": "Other"}
{"value": "724", "type": "Other"}
{"value": "6.773", "type": "Other"}
{"value": "1.94", "type": "Other"}